---
abstract: 'Unconventional superconductors have been long sought for their potential applications in quantum technologies and devices. A key challenge impeding this effort is the difficulty associated with probing and characterizing candidate materials and establishing their order parameter. In this *Letter*, we present a platform that allows us to spectroscopically probe unconventional superconductivity in thin-layer materials *via* the proximity effect. We show that inducing an $s$-wave gap in a sample with an intrinsic $d$-wave instability leads to the formation of bound-states of quasiparticle pairs, which manifest as a collective mode in the $d$-wave channel. This finding provides a way to study the underlying pairing interactions vicariously through the collective mode spectrum of the system. Upon further cooling of the system we observe that this mode softens considerably and may even condense, signaling the onset of time-reversal symmetry breaking superconductivity. Therefore, our proposal also allows for the creation and study of these elusive unconventional states.'
author:
- 'Jonathan B. Curtis'
- 'Nicholas R. Poniatowski'
- Amir Yacoby
- Prineha Narang
bibliography:
- 'references.bib'
title: 'Proximity-induced collective modes in an unconventional superconductor heterostructure'
---

Materials exhibiting unconventional superconductivity are key components of many proposed quantum devices. For instance, triplet superconductors may allow for the incorporation of magnetic functionalities into superconducting electronics, as well as offering larger critical magnetic field strengths @Linder.2015 [@Yang2021]. Similarly, a large amount of work has been devoted towards realizing topological superconductors, such as the elusive chiral $p$-wave state, due to their potential for realizing topologically protected Majorana-based qubits and quantum computation @Alicea_review [@sankar-rmp; @Zareapour.2012]. Many of these useful unconventional states break additional symmetries, beyond global $U(1)$ symmetry, such as time-reversal symmetry @Sigrist2000 [@hirschfeld-s+id; @mixedsymm; @valentin-1; @trsb-review; @Wysokinski.2019].

The question of how to realize @Narang.2020 [@Zareapour.2012] and prepare these systems not withstanding, it is often very difficult to even characterize and verify the nature of these unconventional superconducting phases. Often, low dimensionality, low temperature scales, and complex order parameters can conspire to obscure the microscopic structure of the ground state, making the unambiguous identification of the state challenging. It has recently been emphasized that one potential solution to this problem is to use the spectrum of collective modes in the superconductor to look for signatures of the ground state order @higgs-spect [@higgs-spect2; @poniatowski2021spectroscopic]. For example, one may look at the multiple different Higgs modes of an anisotropic superconductor in order to identify the ground state symmetry @higgs-spect [@nbn-thg; @chiral-higgs; @Nosarzeski.2017]. Similarly, in the case of multicomponent @poniatowski2021spectroscopic [@214-clapping; @Balatsky.2000; @214-clapping] or multiband @multiband-review [@Marciani.2013; @valentin-1] superconductors which break time-reversal symmetry, it has been argued that collective modes associated to the relative phase stiffnesses may also provide signatures of the time-reversal symmetry breaking.

While promising, this method is greatly restricted in its applicability. In order to support these collective modes, the material must already have two or more closely competing interactions, and if the system has a nodal order parameter there is an additional threat due to quasiparticle damping. In addition, the relevant frequency scales for these collective modes is almost always on the order of the electronic gap, and therefore usually falls within a challenging frequency range of low-to-mid THz.

In this *Letter*, we present a way to overcome these challenges in a controlled and tunable manner by using the proximity effect to build a "designer" collective mode. This collective mode can then be used to probe the order parameter of a candidate material by standard means such as Raman or tunneling spectroscopy. Additionally, we show that this protocol may also yield a way to engineer systems which spontaneously breaks time-reversal symmetry, offering a way to systematically study these elusive superconducting states.

![**a.** Schematic of the heterostructure under study in this work: an unconventional superconducting sample placed in proximity to a conventional bulk superconducting substrate. The two sub-systems are coupled via single-particle tunneling which occurs at the rate $\gamma$. **b.** Phase diagram of the system. Below $T_s$, the substrate is superconducting and induces a minigap in the sample via the proximity effect. When this minigap becomes large enough, it converts the overdamped fluctuations of the $d$-wave superconducting order into a sharp collective mode. As the sample transition temperature $T_d$ is approached, this proximitized collective mode softens and ultimately condenses out-of-phase with the substrate order parameter, spontaneously breaking time-reversal symmetry. Below $T_d$, the proximity-induced collective mode becomes the usual clapping mode in time-reversal symmetry breaking superconductors. <span data-label="fig:overview"></span>](bs-overview.pdf){width="\linewidth"}

Fundamentally, our scheme relies on using a bulk "substrate" $s$-wave superconductor to proximity induce $s$-wave superconductivity in a thin "sample" layer of unconventional superconductor which has an intrinsic instability towards pairing in a non-$s$-wave channel, as depicted in Fig. \[fig:overview\](a). In the presence of the proximity-induced minigap this residual interaction manifests through the formation of stable bound-states of pairs of quasiparticles. These bound states essentially realize the Bardasis-Schrieffer, or "particle-particle exciton," collective mode @bs-modes, but in this case the sub-dominant pairing interaction is the dominant pairing interaction in the sample.

More generally, this realizes a scenario where the substrate and sample order parameters are "competing" @hirschfeld-s+id [@mixedsymm]. If the intrinsic pairing interaction in the sample is sufficiently strong then the particle-particle bound-state may itself condense, at which point we show the system will undergo a second phase transition into a state with mixed order in the two channels, and that this will spontaneously break time-reversal symmetry. This hierarchy of temperatures and the various regimes are shown in Fig. \[fig:overview\](b).

For specificity, we will demonstrate this idea by considering a concrete model where the sample has single-band spin-singlet $d_{x^2 - y^2}$-wave order, though many of our results are expected to generalize to more complex sample order parameters. For simplicity, we take the sample thickness to be thin compared to the coherence length in the out-of-plane direction, such that we may neglect the dispersion in this direction, and hence neglect the spatial dependence of the problem in the transverse direction.

In this case, we describe the intrinsic pairing interaction in the sample by a BCS Hamiltonian $$\begin{gathered}
\label{eqn:sample-H}
    H_{0} = \sum_{\bf p \sigma } \xi_{\bf p} c_{\bf p\sigma}^\dagger c_{\bf p\sigma } \\
    - g_d \sum_{\bf q}\int_{\bf p,p'} \chi^d_{\bf p}\chi^d_{\bf p'} c_{\mathbf{p}'+\frac12\mathbf{q},\uparrow }^\dagger c_{-\mathbf{p}'+\frac12\mathbf{q},\downarrow }^\dagger c_{-\mathbf{p}+\frac12\mathbf{q}\downarrow} c_{\mathbf{p}+\frac12\mathbf{q} \uparrow} ,\end{gathered}$$ with the dispersion relation $\xi_{\bf p} = \mathbf{p}^2 /2m - E_F$ and $d$-wave form-factor $\chi^d_{\bf p} = \sqrt{2}\cos(2\theta_{\bf p})$ (the momentum angle is measured from the $x$-axis, ultimately set by the crystal lattice). The second term describes the scattering of Cooper pairs with center-of-mass momentum $\bf q$ and relative momentum $\bf p$, and in particular projects the interaction onto the $d$-wave singlet channel.

Within mean-field theory the pairing interaction can be decoupled, yielding the standard Bogoliubov-de Gennes Hamiltonian for quasiparticles. Solving this self-consistently for the $d$-wave gap $$\label{eqn:d-wave-gap}
    \frac{1}{g_{d}} \Delta^d = \int_{\bf p} \chi^d_{\bf p} \langle c_{-\bf p \downarrow} c_{\bf p \uparrow} \rangle ,$$ we find that $d$-wave pairing sets in at a temperature $T_d^{(0)}$ which is given by the standard BCS formula in terms of the dimensionless pairing strength $\lambda_d = g_d \nu_F $ (with $\nu_F$ the density-of-states at the Fermi level), and a UV cutoff $\Lambda$ of order of the characteristic frequency of whatever mediates pairing in the sample (for phonons this is the standard Debye frequency). In this work we do not consider any changes to the intrinsic interaction due to the substrate, though relaxing this is an interesting direction for future study.

We now introduce the coupling to the substrate, which we treat as a fixed "reservoir," that doesn't experience any back-reaction due to the coupling to the sample. In particular, we assume the substrate is much thicker than the sample and the $s$-wave coherence length. Crucially, we also assume that the substrate transition temperature $T_s$ is much larger than the intrinsic transition temperature in the sample $T_d^{(0)}$, or equivalently that the substrate superconducting gap $|\Delta_s|$ has largely saturated once the temperature reaches $T \sim T_d^{(0)}$.

We assume a local tunneling in to the substrate with effective tunneling matrix element $\mathfrak{t}$. At second-order we find the tunneling energy scale $\gamma = 2\pi \nu_s |\mathfrak{t}|^2$, where $\nu_s$ is the density-of-states in the substrate (for details see Supplemental Material). We largely focus on the regime $\Delta_s \gg \gamma$, such that the tunneling scale is less than the substrate gap (for a less restrictive treatment, see Supplemental Material) and we may treat processes only in the Andreev channel.

Provided the substrate superconducting phase is not strongly fluctuating (the relevant energy and length scales over which the phase varies are the plasma frequency and the in-plane penetration depth of the substrate, respectively), we can model the proximity-induced superconducting gap in the sample by adding a term to the Hamiltonian (see Supplemental Material for derivation), $$\label{eqn:prox}
    H_{\rm prox} = -\frac12 \gamma \sum_{\bf p}  c_{-\bf p\downarrow } c_{\bf p \uparrow } \frac{\overline{\Delta_s} }{|\Delta_s|} + c_{\bf p\uparrow }^\dagger c_{-\bf p \downarrow }^\dagger \frac{\Delta_s}{|\Delta_s|}.$$ In particular, this opens a minigap at the Fermi level for the electrons in the sample (in the Andreev regime $|\Delta_s| \gg \gamma$, the size of the minigap is $\gamma/2$) and the phase is referenced with respect to the substrate phase. We henceforth set this phase to be zero, such that the substrate gap is taken to be real and positive.

Since the proximity effect opens a gap on the Fermi surface of the sample, we expect the intrinsic $d$-wave pairing transition to be suppressed. Indeed, by solving the mean-field equations in the $d$-wave channel and incorporating the new proximity gap, we find that there is a depression of the critical temperature to $T_d < T_d^{(0)}$. These results are summarized in Fig. \[fig:tc\]a, where we use the frequency-dependent Matsubara Green's function, derived in the Supplemental Material, to solve Eq.  and identify the critical temperature in the $d$-wave channel.

We now proceed to our main result, which is the emergence of the bound-state collective mode. Above the new $d$-wave transition temperature, the $d$-wave order is uncondensed but still fluctuates due to the remnant pairing interaction. Within the Random Phase Approximation we may derive an equation of motion which describes the dynamics of this fluctuating $d$-wave order. This is derived in detail in the Supplemental Material, but it may be understood as the linear-response pair-susceptibility of the sample in the proximitized state @Scalapino.1970. The presence of a bound-state collective mode then shows up as a resonance in the pair-susceptibility.

We separate the $d$-wave order parameter into the components which are in-phase and out-of-phase with respect to the substrate condensate, writing $\Delta^d_{\bf q}(t) = h_{\bf q}(t) + i d_{\bf q}(t)$. We find that the in-phase component $h_{\bf q}$ has no sharp resonance and essentially mirrors the two-particle continuum, and thus we will henceforth neglect the in-phase component. This is in line with the expectation that the $s$- and $d$-wave orders are competing and therefore the "repulsion" between the two orders is minimized when they are mutually out of phase @mixedsymm.

At linear order we calculate the spectral function for the dynamic pair-susceptibility in the out-of-phase fluctuation $d_{\bf q}$ channel $$\mathcal{A}_{dd}(\Omega,{\bf q}) = -\frac{1}{\pi}\Im\left\{ -i \int_0^{\infty}dt e^{i\Omega t} \langle [ d_{\bf q}(t), d_{-\bf q}(0)]\rangle \right\} ,$$ which in particular captures the binding energy and linewidth of the $d$-wave excitation. The spectral function $\mathcal{A}_{dd}(\Omega,{\bf q})$ is obtained in the Supplemental Material in terms of the Nambu-Gor'kov Green's functions using the Keldysh technique, although it may also be calculated using, e.g. the Anderson pseudo-spin method provided $|\Delta_s | \gg \gamma$, so that retardation and damping due to the substrate may be safely neglected.

![Evolution of the collective mode spectral function with temperature. We fix the tunneling strength $\gamma = .2$ meV and substrate gap to be $\Delta_s = 1.0$ meV, and hold the cutoff $\Lambda = 30$ meV and BCS constant $\lambda^{-1}_d = 4.58658$, corresponding to an intrinsic critical temperature of $T_d^{(0)} = .344$ meV. The finite $\gamma$ leads to a reduced critical temperature of $T_d = .282$ meV, giving ratio $T_d^{(0)} \sim 1.2 T_d$. **a.** The collective mode spectral function for temperatures between $T_d$ and $1.4\, T_d$, from which we see that the spectral peak of the mode sharpens and progressively softens as the temperature is lowered. At $T = T_d$, the mode ultimately softens to zero frequency. **b.** The spectral function for $T/T_d = 1, 1.1, 1.2, 1.3, 1.4$. We see that the mode clearly separates from the quasiparticle continuum below $T \lesssim T_d^{(0)}$, and softens completely at $T_d$.<span data-label="fig:bs-temp"></span>](bs-temp.pdf){width="\linewidth"}

We present the spectral function $\mathcal{A}_{dd}(\Omega,\mathbf{q}=0)$ in Fig. \[fig:bs-temp\] for different temperatures $T\geq T_d$ at fixed $\gamma, \Delta_s,T_d^{(0)}$. At high temperatures, we see no clear distinction between the collective mode and the bottom of the quasiparticle continuum. Lowering the temperature reduces thermal broadening and pulls the mode out of the continuum, yielding a sharp collective mode which resides within the proximity-induced minigap. This occurs once the temperature $T \sim T_d^{(0)}$, the characteristic temperature scale of the intrinsic pairing interactions. As we decrease the temperature further the mode continues to soften. Remarkably, at $T = T_d<T_d^{(0)}$ the mode softens completely, and we see the $d$-wave bound-state itself condenses. As we now demonstrate, this signals the onset of a second phase transition into a state with finite $d$-wave order.

![**a.** Transition temperature $T_d$ of the sample as a function of the dimensionless $d$-wave coupling constant $\lambda_d = \nu_F g_d$, plotted for different values of the tunneling rate $\gamma$. Notice that for any fixed $\lambda_d$, $T_d$ is suppressed as the tunneling rate is increased. **b.** Temperature dependence of the quadratic coefficients in the Ginzburg-Landau expansion for $h$ and $d$. The change of sign of each coefficient signals condensation in that channel, and one sees that the out-of-phase $d$ mode condenses first. **c.** Amplitude of the sample order parameter $\Delta^d = i\langle d \rangle$ near $T_d$. Inset: illustration of the relative Higgs and Bardasis-Schreiffer modes, and their phase relative to the $s$-wave substrate order parameter<span data-label="fig:tc"></span>](bs-tc.pdf){width="\linewidth"}

In fact, this split transition behavior is a generic feature of systems with strongly competing superconducting orders, and in this case it signals the onset of time-reversal symmetry breaking @Sigrist2000 [@hirschfeld-s+id; @mixedsymm]. This is understood by noting that the collective mode is in the out-of-phase channel, and therefore it is odd under time-reversal symmetry. Condensing this mode requires spontaneously choosing the relative phase to be either $+\pi/2$ or $-\pi/2$, entering into either an $s+id$ or $s-id$ state @hirschfeld-s+id [@mixedsymm].

This intuition is confirmed by explicitly solving the Ginzburg-Landau mean-field equation for the $d$-mode as we pass through the temperature $T_d$. Expanding the gap equation Eq. \[eqn:d-wave-gap\] for small $\Delta_d$ we obtain an equation for the static, homogeneous component of $d_{q=0} \equiv d$ (see Supplemental Material) of $$\left(r_d + u_d d^2 \right) d = 0 .$$ The coefficients $r_d  \sim T - T_d $ and $u_d\sim 1/T^2$ @agd, as well as the quadratic Ginzburg-Landau coefficient for the amplitude mode $r_h$ are calculated microscopically in the Supplemental Material. In Fig. \[fig:tc\](b), we plot the coefficient $r_d$ alongside $r_h$ and see explicitly that $r_d$ changes sign first at $T = T_d$, confirm our inference based on the collective mode spectrum. Below $T_d$ the order parameter $d$ acquires a non-zero value shown explicitly in Fig. \[fig:tc\](c). Note this transition does not spontaneously break $U(1)$ symmetry, which has already been broken by the substrate order parameter, but it does break the remnant $\mathbb{Z}_2$ symmetry, under which $id \to - id $.

The breaking of time-reversal symmetry in such an "$s$-$d$" heterostructure has already been predicted, for instance at the twin-grain boundaries in cuprate systems @sigrist-s-d [@sigrist-trsb-3; @sigrist-trsb-2], at the interface of "$s$-$d$" superconductors @Huck.1997 [@sigrist-trsb-1; @Lin.2012], and between twisted cuprate layers @twisted-bscco [@twisted-bscco-2; @Zhao.2021]. Our calculation seems to indicate that the breaking of time-reversal symmetry in these systems is in some sense the "final fate" of what we have discussed here, and in particular the breaking of time-reversal symmetry in these systems ought to be heralded by a softening collective mode, as we have shown. It is also worth commenting that, just as we have shown the Bardasis-Schrieffer collective mode emerges in the normal state of the heterostructure, we may also expect a new collective mode to emerge once time-reversal symmetry is broken below $T_d$ @poniatowski2021spectroscopic [@214-clapping; @Balatsky.2000; @Marciani.2013], thereby making connection to previous proposals for collective-mode spectroscopy.

![Spectral function of proximity-induced Bardasis-Schrieffer collective mode for different strengths of the tunneling-induced minigap. We fix the substrate gap to be $\Delta_s = 1.0$ meV, and hold the cutoff $\Lambda = 30$ meV and BCS constant $\lambda^{-1}_d = 4.58658$, corresponding to an intrinsic critical temperature of $T_d^{(0)} = .344$ meV. We also fix the temperature $T = T_d^{(0)}$. We then study the spectral functions while we vary the size of the tunneling rate $\gamma$ from $.1$meV in (a) through $.4$meV in (d) in increments of $.1$ meV. The plots are made over a frequency range from $0$ to $2\gamma$, and at $\Omega = \gamma$ we place a line as a guide to the eye, which indicates where the two-particle continuum formally begins. <span data-label="fig:bs-gamma"></span>](bs-gamma.pdf){width="\linewidth"}

Before concluding we study the dependence of the collective mode found in Fig. \[fig:bs-temp\] upon the minigap $\gamma$. The minigap $\gamma$ is crucial for the existence of the collective mode, as otherwise it would be overdamped by the quasiparticle continuum. In Fig. \[fig:bs-gamma\] we illustrate this explicitly by plotting the spectral function $\mathcal{A}_{dd}(\Omega,\mathbf{q}=0)$ for a variety of tunneling strengths $\gamma$ at fixed temperature $T = T_d^{(0)}$ and substrate gap $\Delta_s$. For small minigap $\gamma$, seen in Fig. \[fig:bs-gamma\](a), we see the collective mode is indistinguishable from the quasiparticle continuum[^1]. Proceeding to larger values of $\gamma$, e.g. in Fig. \[fig:bs-gamma\](c),(d), we see a well separated mode appears within the minigap. Practically, this points to the necessity of establishing good electrical contact between the sample and substrate, so that the tunneling scale, and therefore minigap $\gamma$, is as large as possible.

We also briefly comment here on the $\Delta_s$ dependence of the mode, which is studied in the Supplementary Material. In particular, we see that at finite $\gamma$ and small $\Delta_s$ the substrate acts as an incoherent reservoir. In this case we recover the known behavior for overdamped fluctuations of the sample's superconducting order @larkin-book, with the $d$-wave pairs decaying with a characteristic lifetime $\tau \sim 1/(T - T_d)$, thereby also allowing for the study of critical superconducting fluctuations @Scalapino.1970 [@Kadin.1982; @Goldman.2006]. Nevertheless, for the purposes outlined in this work, we see that it is beneficial for the substrate to have as large a gap as possible. We now briefly discuss various experimental signatures of this mode.

The first is electron tunneling spectroscopy @Wolf. In inelastic tunneling spectroscopy, bosonic excitations such as phonons @Vitali.2004 and magnons @Balashov.2006 are routinely observed by studying characteristic $I-V$ curves. In particular, these bosonic excitations may appear as a sharp feature in $d^2I/dV^2$, which signals the opening of a new inelastic scattering channel for electrons at that bias energy. In this context, we may imagine it is also possible for an electron to emit a collective mode in the process of tunneling in to the sample, and therefore we should also expect a similar kink feature to appear in the $I-V$ curve once the energy passes the collective mode threshold. While this is still a relatively difficult measurement to perform, there is some precedent for using this technique to study collective modes of unconventional superconductors @Hlobil.2017 [@Jandke.2016]. Since, as we have seen, the collective mode we identify here can have strong temperature dependence, this may help to identify such a feature since it in principle will soften considerable as the temperature is lowered.

In a similar vein, it may also be possible to identify this collective mode using ARPES, in which case the mode will again manifest as an inelastic contribution to the electronic self-energy @Norman.1999 [@Valla.1999; @Hoffman.2009]. In this context, ARPES has the additional benefit of potentially observing the momentum dependence of the coupling, which could help identify the symmetry channel of the collective mode, and therefore identify the symmetry channel of the underlying pairing interaction.

Lastly, we also expect Raman spectroscopy to be sensitive to the collective mode. This is not surprising since it has long been known that the Bardasis-Schrieffer mode, when it exists, is a Raman active mode @bs-raman [@Devereaux.2007; @Scalapino.2009]. Like ARPES, Raman spectroscopy also has the potential to probe the selection rules of the collective mode in addition to the frequency of the mode.

Finally, we discuss promising materials for the realization of this proposal. In our model, we considered a $d$-wave system but this is not crucial; much of what we assumed only relied on the sample order parameter being orthogonal to the $s$-wave substrate order. However, we do want the intrinsic critical temperature $T_d^{(0)}$ to be low compared to the bulk transition temperature of the substrate, $T_s$.

There are a number of interesting van der Waals compounds @Zhou.2016 [@Wakatsuki.2016], such as MoS$_2$ @Lu.2015 [@Saito.2016], NbSe$_2$ @Xi.2016, WS$_2$ @Lu.2018, and WTe$_2$ @wte2 [@wte2-1; @fu-wte2] which exhibit possibly unconventional superconductivity and can be exfoliated into thin layers. In addition, moiré bilayer and trilayer graphene quite likely exhibit unconventional superconductivity at a low temperature scale and are also easily exfoliated @bilayer-1 [@trilayer-1; @bilayer-stm; @trilayer-stm].

It may also be possible to study this physics using a severely overdoped cuprate, provided the transition temperature can be depressed below that of a realistic $s$-wave system. This has the benefit of having an established gap-symmetry and therefore may offer a useful test-case. In addition, recent efforts have established that certain cuprates may also be prepared in thin layers, or even single copper-oxide layers @Yu.2019. In this context, our proposal has some technical overlap with recent proposals for time-reversal symmetry breaking chiral superconductivity in systems of twisted cuprate monolayers @twisted-bscco [@twisted-bscco-2; @Zhao.2021].

The main limitation is the requirement that the $s$-wave substrate superconductor have a higher critical temperature than the sample. To maximize the substrate transition temperature, the most likely candidate substrates are then Nb, NbN, or NbTiN, with $T_s\sim 7-15$ K. It may also be possible to use a fullerene such as Rb$_3$C$_{60}$, which would allow one to access higher temperatures $T_s \sim 30$K, at the expense of likely introducing other complications @Tanigaki.1991.

It would be interesting to try and apply our results to sample superconductors which already feature intrinsic collective modes but which are overdamped, e.g. due to nodal quasiparticles. By opening a proximity-induced gap, one may attempt to, e.g. stabilize the Higgs collective mode, which is usually located at the gap edge and subject to quasiparticle damping @higgs-cdf. In this way, much like a charge-density wave order parameter can separate the Higgs mode from the continuum and enable its coherent oscillation @higgs-arcmp [@varma-cdw; @higgs-cdw], it might also be possible to use the small proximity-induced gap to separate the continuum from the Higgs mode and enable its widespread detection.

In conclusion, we have considered a simple model of an unconventional superconducting sample that is proximitized by a dominant $s$-wave superconducting substrate and seen that this can lead to a sharp collective mode which captures the intrinsic pairing interaction in the sample. This then greatly expands the platforms for studying unconventional superconductivity through their collective modes and increases the number of experimentally accessible probes for these difficult to characterize states.

Acknowledgements
================

We acknowledge useful discussions with Eugene Demler, Stuart S.P. Parkin, Manfred Sigrist, Matteo Mitrano, Ken Burch, Zachary Raines, Andrew Allocca, Niels Schröter, and Mostafa Marzouk. N.R.P. and J.B.C. acknowledge the hospitality of the ETH Zürich Institute for Theoretical Physics and the Max Planck Institute for the Structure and Dynamics of Matter (MPSD, Hamburg), where part of this work was completed. This work was primarily supported by the Quantum Science Center (QSC), a National Quantum Information Science Research Center of the U.S. Department of Energy (DOE). J.B.C. is an HQI Prize Postdoctoral Fellow and gratefully acknowledges support from the Harvard Quantum Initiative. N.R.P. is supported by the Army Research Office through an NDSEG fellowship. A.Y. is partly supported by the Gordon and Betty Moore Foundation through Grant GBMF 9468 and by the National Science Foundation under Grant No. DMR-1708688. P.N. is grateful for the hospitality of the Max Planck Institute for the Structure and Dynamics of Matter where part of this work was completed supported by a Max Planck Sabbatical Award and a Bessel Research Award of the Alexander von Humboldt Foundation. P.N. is a Moore Inventor Fellow and gratefully acknowledges support through Grant GBMF8048 from the Gordon and Betty Moore Foundation.

[^1]: In particular, in the mean-field limit the two-particle spectral function is completely fixed by the single-particle density-of-states, and this exhibits a weak singularity at the gap edge which may be confused with a collective mode if the resonance lies to close to the continuum.

{'source': 'arXiv_out/2201'}